Nanocomposite Coatings: Preparation, Characterization ... matrix, these nanocomposite coatings could
Embed Size (px)
Transcript of Nanocomposite Coatings: Preparation, Characterization ... matrix, these nanocomposite coatings could
Review Article Nanocomposite Coatings: Preparation, Characterization, Properties, and Applications
Phuong Nguyen-Tri ,1 Tuan Anh Nguyen ,2 Pascal Carriere,3 and Cuong Ngo Xuan4
1Department of Chemistry, University of Montréal, Montréal, QC, Canada 2Institute for Tropical Technology, Vietnam Academy of Science and Technology, Hanoi, Vietnam 3Laboratoire MAPIEM (EA 4323), Matériaux Polymères Interfaces Environnement Marin, Université de Toulon, Toulon, France 4National Key Laboratory for Welding and Surface Treatment Technologies, National Research Institute of Mechanical Engineering, Hanoi, Vietnam
Correspondence should be addressed to Phuong Nguyen-Tri; email@example.com
Received 9 September 2017; Revised 12 December 2017; Accepted 15 January 2018; Published 13 February 2018
Academic Editor: Omar S. Es-Said
Copyright © 2018 Phuong Nguyen-Tri et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
Incorporation of nanofillers into the organic coatings might enhance their barrier performance, by decreasing the porosity and zigzagging the diffusion path for deleterious species. Thus, the coatings containing nanofillers are expected to have significant barrier properties for corrosion protection and reduce the trend for the coating to blister or delaminate. On the other hand, high hardness could be obtained for metallic coatings by producing the hard nanocrystalline phases within a metallic matrix. This article presents a review on recent development of nanocomposite coatings, providing an overview of nanocomposite coatings in various aspects dealing with the classification, preparative method, the nanocomposite coating properties, and characterization methods. It covers potential applications in areas such as the anticorrosion, antiwear, superhydrophobic area, self-cleaning, antifouling/antibacterial area, and electronics. Finally, conclusion and future trends will be also reported.
1.1. Definition. A nanocomposite coating is a material com- posed of at least two immiscible phases, separated from one another by interface region. The material must contain the nanometer scale in at least one dimension in which themajor component is called matrix in which fillers are dispersed .
1.2. Classification. The classification of nanocomposite coat- ings is based on various methods dealing with (i) type of nanostructured fillers or (ii) type of matrix where filler nanostructures are dispersed.
1.2.1. Type of Nanostructured Fillers. There are 3 main groups of nanocomposite coating as follows :
(i) 0D nanocomposite coatings: the filler are nanoparti- cles (3 dimensions in nanometer scale).
(ii) 1D nanocomposite coatings: the filler are nanotubes or whiskers (2 dimensions in nanometer scale).
(iii) 2D nanocomposite coatings: the filler are nanolayers (1 dimension in nanometer scale).
1.2.2. Type of Matrix. Tow types of matrix which are organic and inorganic matrix can be found. Thus, there are 4 main groups of nanocomposite coating as follows (matrix/ nanofiller):
(i) Organic/inorganic nanocomposite coatings (O/I na- nocomposite coatings)
(ii) Organic/organic nanocomposite coatings (O/O na- nocomposite coatings)
(iii) Inorganic/organic nanocomposite coatings (I/O na- nocomposite coatings)
(iv) Inorganic/inorganic nanocomposite coatings (I/I na- nocomposite coatings).
Hindawi International Journal of Corrosion Volume 2018, Article ID 4749501, 19 pages https://doi.org/10.1155/2018/4749501
http://orcid.org/0000-0001-6578-5716 http://orcid.org/0000-0003-4445-4154 https://doi.org/10.1155/2018/4749501
2 International Journal of Corrosion
Dip coating Spin coating Electrodeposition
Figure 1: Preparation of coatings by sol-gel method .
1.3. Materials 1.3.1. Materials for Matrix. For organic matrix, called poly- mer-based nanocomposite, the most used polymers for prep- aration of nanocomposite coating can be listed as follows: epoxy [2–7], polyurethane [8, 9], Chitosan [10, 11], polyethy- lene glycol (PEG) [12–15], polyvinylidene fluoride (PVDF) , PANi [17–19], PPy [20–23], polystyrene , polyamic acid and polyimide , rubber-modified polybenzoxazine (PBZ) , polymers containing reactive trimethoxysilyl (TMOS) , pullulan , fluoroacrylic polymer [29, 30], ethylene tetrafluoroethylene (ETFE) , polyacrylate , poly(N-vinyl carbazole) , polycarbonate , fluorinated polysiloxane , polyester , polyacrylic , polyvinyl alcohol (PVA) , polydimethylsiloxane , polyamide , and UV-curable polymers .
For inorganic matrix, such as metal matrix or alloy matrix, these nanocomposite coatings could be prepared by various methods, including chemical vapor deposition (CVD) (see Figure 3), powder metallurgy, physical vapor deposition (PVD) [41–45], thermal plasma spray [46–48], sol-gel [49–52] (see Figure 1), epitaxial growth , cold spray
[54–61] (see Figure 2), and electrodeposition [62–67]. Metal matrix composite coatings that dispersed a second phase [68, 69] have attracted extensive attention owing to unique properties such as oxidation and corrosion resistance [69, 70], wear resistance [71, 72], and magnetic properties .
1.3.2. Materials for Nanofillers. For inorganic nanofillers, the types of nanoparticles are carbides , nitrites [59–61, 73–77], borides , oxides [4, 5, 62, 65], metallic particles [17, 78], clay [4, 5, 35], CNT , and nanodiamond [56, 79]. For organic nanoparticles (organic nanofiller), the most used nanoparticles were PTFE [80–82], PEO , PANi , or nanocellulose and cellulose nanocrystal [18, 40].
2. Preparative Methods
2.1. Sol-Gel Method. The sol-gel method is suitable to obtain high quality films up to micron thickness and is a com- plementary of the physical deposition techniques. However, there are limits of sol-gel application to coating on the metallic subtracts. This method exhibits several drawbacks involving crackability and thickness limits. Sometimes also
International Journal of Corrosion 3
High pressure gas supply
Control panel High pressurepowder feeder
Accelerating gas line heater
de Laval nozzle
N2 N2 N2 N2
Figure 2: Principle of cold spray technique for preparation of nanocomposite .
Plasma deposition O
Figure 3: Plasma enhanced chemical vapor deposition .
the thermal treatmentmay be critical. Tensile stresses develop during drying and can lead to crack formation if the film is thicker than a critical value.
In case of inorganic matrix, the second phase can be added to sol-gel for inorganic nanofillers, such as the I/I coatings [49–52]. In the case of organic matrix, a well- known approach to generate inorganic nanophases within an organic matrix is to utilize sol-gel chemistry . Inorganic sol-gel precursors such as silicon, titanium, aluminum, and zirconium metal alkoxides are employed in the formulation of nanocomposite coatings. A wide range of oligomers as well as low molecular weight organic compounds are often reported to be used as organic phase precursors. Under controlled conditions, silanes and organic molecules can form coatings containing silica nanoparticles or nanophases. In the presence of a coupling agent, the organic and inorganic phases can be covalently linked. Silica nanofiber forma- tion in a system containing TEOS, methacryloxypropyl- trimethoxysilane (MAPTMS), a urethane acrylate resin, and an acrylated phenylphosphine oxide oligomer (APPO) has been reported .
The nanofibers were shown to improve the mechanical properties of the organicmatrix. By this sol-gel process, Facio andMosquera  also successfully fabricated the nanocom- posite coatings containing (i) a mixture of monomeric and oligomeric ethoxysilanes, (ii) a hydroxyl-terminated poly- dimethylsiloxane, (iii) colloidal silica particles, and (iv) a surfactant (n-octylamine). In addition, the sol-gel method could be used in combination with the electrodeposition for incorporation of inorganic nanofillers into the organicmatrix  or into inorganic matrix .
2.2. Cold Spray Method. Unlike the traditional thermal spray (gas-flame, plasma, and detonation spraying), cold spraying allows fabrication of coatings at the lower temperatures than melting points of the sprayedmaterials. Cold spray technique was conducted at low temperatures, so thismethod avoids the deterioration phenomenon of the materials such as oxidation and decomposition as well as phase transition during the process. The obtained coatings have low porosity (280MPa) and strong adhesion (>70MPa).
This method is used to produce the nanocomposite coating, which has metallic matrix, such as Cu [54, 55], Al [56, 57], Co , or alloy matrix [59–61], and its nanofillers are nitrite, carbide, boride, diamond, CNT, or others [54–61]. To fabricate the nanocomposite powders for this cold spray method, the mechanical alloying (MA) should be used with metallic matrix powders and other nanoparticles.
2.3. CVD Method. This method usually used for the fabri- cating of the I/I